Infiltration liquid crystal in microstructured polymer optical fibers · Microstructured polymer...
Embed Size (px)
Transcript of Infiltration liquid crystal in microstructured polymer optical fibers · Microstructured polymer...
General rights Copyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright owners and it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights.
Users may download and print one copy of any publication from the public portal for the purpose of private study or research.
You may not further distribute the material or use it for any profit-making activity or commercial gain
You may freely distribute the URL identifying the publication in the public portal If you believe that this document breaches copyright please contact us providing details, and we will remove access to the work immediately and investigate your claim.
Downloaded from orbit.dtu.dk on: Aug 08, 2021
Infiltration liquid crystal in microstructured polymer optical fibers
Yuan, Scott Wu; Wei, Lei; Bang, Ole
Published in:Conference proceedings, CLEO/Europe - EQEC
Link to article, DOI:10.1109/CLEOE-EQEC.2009.5192749
Document VersionPublisher's PDF, also known as Version of record
Link back to DTU Orbit
Citation (APA):Yuan, S. W., Wei, L., & Bang, O. (2009). Infiltration liquid crystal in microstructured polymer optical fibers. InConference proceedings, CLEO/Europe - EQEC IEEE. https://doi.org/10.1109/CLEOE-EQEC.2009.5192749
Infiltration Liquid Crystal in Microstructured Polymer Optical Fibers
W. Yuan), L. wei, o. Bani1. DTU Fotonik, Dept. ofPhotonics Engineering, Technical University ofDenmark, DK-2800 Kgs. Lyngby, Denmark
Microstructured polymer optical fibres (mPOFs) have attracted significant interests , mainly because fabricationtechniques have allowed novel structures to be made at low temperature with polymers, especially PMMA(refractive index 1.49) . Recently, thermal and electrical tunabilities of liquid crystals infiltrated silicaphotonic bandgap fibres have been demonstrated, and various devices have also been developed [2, 3].
Here, to our knowledge, we firstly demonstrate the photonic bandgap effect with PMMA mPOF by filling theair holes with liquid crystal , and subsequently change the light guidance mechanism from index guiding tobandgap guiding. The triangular structure PMMA mPOF used in the experiment is fabricated by our group withdiameter 130Jllll and a solid core surrounded by 3 rings of air holes , as shown in Fig. I(a) the air hole diameterand hole to hole pitch are 4.5Jl1ll and IOum, respectively. A 60cm length mPOF is butt-coupled to aconventional single mode fiber (SMF) with the broadband light from a supercontinuum source (SuperK, KoherasA/S). The guided modes image under 50X microscope is shown in Fig. 1(b). It is clear to see the colour of theguided modes is red, since some wavelengths are attenuated by the material loss of PMMA in visible region. Apositive dielectric anisotropy liquid crystal E7 (Merck, Germany, no=1.52, Ile=1.74) is then infiltrated into about6cm of the length of mPOF by using capillary forces with the duration of 45 minutes. The end of mPOF whereliquid crystal is filled is then butt-coupled again with SMF. After liquid crystal infiltration, the guided modesimage is shown in Fig. I(c) , and it is found the colour of the guided modes is changed from red to green, whichmeans some wavelengths in red region have been filtered out due to the bandgap effect induced by liquid crystal.The transmission spectrum is measured by an optical spectrum analyzer with lnm resolution, and normalized to that ofthe unfilled fiber as shown by the solid line in Fig. 1(d). The difference of spectra of Fig. 1(d) clearly reveals that,by filling the liquid crystal, some new bandgaps are formed in the wavelength range of 730nm-780nm, which isquite different with the material loss spectrum shown as the black dash line.
The possibility of applying mPOF to fabricate turnable fiber devices will make mPOF as an ideal substitutionof the expensive silica photonic crystal fibers in practical applications. More investigations will be done in nearfuture, e.g. thermal and electrical tunabilities.
Fig. 1 (a). The cross section of the mPOF used in this experiment. (b) The guided modes image of unfilled mPOF withthe broadband light from a supercontinuum source. (c) The guided modes image of E7 filled mPOF. (d) Transmissionspectrum of liquid crystal filled mPOF (the solid line) and material loss spectrum ofmPOF (the dash line).
References[11M. Large, L. Poladian , G. Barton, M. Eijkelenborg, "Microstructured polymer optical fibres," Springer, (2008). T. T. Alkeskjold, L. Scolari, D. Noordegraaf, 1. Laegsgaard , 1. Weirich, L. Wei, G. Tartarini , P. Bassi, S.Gauza, S. Wu, A. Bjarklev,"Integrating liquid crystal based optical devices in photonic cystal fibers," Opt. Quant. Electron. 39, 1009 (2007). L. Wei, L. Eskildsen, J. Weirich, L. Scolar i, 1. 1. Alkeskjold , and A. Bjarklev , "Continuously tunable all-in-fiber devices based onthermal and electrical control of negative dielectric anisotropy liquid crystal photonic bandgap fibers," App!. Opt. 48,497-503 (2009).
978-1-4244-4080-1/09/$25.00 @2009 IEEE
Authorized licensed use limited to: Danmarks Tekniske Informationscenter. Downloaded on October 28, 2009 at 08:48 from IEEE Xplore. Restrictions apply.